Research Article  Open Access
Tao Ma, Yao Zhang, Hao Wang, Xiaoming Huang, Yongli Zhao, "Influences by Air Voids on the LowTemperature Cracking Property of DenseGraded Asphalt Concrete Based on Micromechanical Modeling", Advances in Materials Science and Engineering, vol. 2016, Article ID 6942696, 10 pages, 2016. https://doi.org/10.1155/2016/6942696
Influences by Air Voids on the LowTemperature Cracking Property of DenseGraded Asphalt Concrete Based on Micromechanical Modeling
Abstract
This study characterized the impacts of air voids on the lowtemperature cracking behavior of densegraded asphalt concrete. Virtual lowtemperature bending beam test for densegraded asphalt concrete was built and executed by discrete element method and PFC3D (particle flow code in three dimensions). Virtual tests were applied to analyze the impacts by content, distribution, and size of air voids on the lowtemperature properties of densegraded asphalt concrete. The results revealed that higher air void content results in worse lowtemperature property of densegraded asphalt concrete, especially when the air void content exceeds the designed air content; even with the same designed air void content, different distributing condition of air voids within asphalt concrete leads to different lowtemperature properties of asphalt concrete, especially when the air void content in the centrallower part of testing sample varies. Bigger size of single air void which tends to form interconnected air voids within asphalt concrete has more harmful impacts on the lowtemperature properties of asphalt concrete. Thus, to achieve satisfied lowtemperature properties of densegraded asphalt concrete, it is critical to ensure the designed air void content, improve the distribution of air voids, and reduce the interconnected air voids for densegraded asphalt concrete.
1. Introduction
Lowtemperature cracking is one of the main diseases of asphalt pavement especially in cold weather. Since asphalt concrete is typical heterogeneous composite materials, the composition ratios of different constituents within asphalt concrete and their microstructure distribution have important influences on the cracking behavior of asphalt concrete [1, 2]. However, laboratory tests cannot fully evaluate the influences by different constituents of asphalt concrete on its cracking behavior [3]. Although finite element method can well depict the cracking behavior of asphalt concrete, it still has difficulties to characterize the heterogeneity of asphalt concrete and depict the microstructure of different constituents of asphalt concrete [4–8]. The discrete element method proposed by Cundall can evaluate the interacting behavior within discrete particles by characterizing the translational and rational movements of different particles based on Newton’s second law of motion and a finite difference scheme [9, 10]. It provides a more promising way to model and describe the heterogeneous microstructure and micromechanical behavior of asphalt concrete.
After contactbonding relationships for asphalt concrete were built, DEM has been extensively used to characterize the performances of asphalt concrete. Although many different discrete element software have been developed, the particle flow code in two and three dimensions (PFC2D/3D) was used most popularly for asphalt concrete analysis due to its good modeling productivity and flexible capacity to characterize the moving behavior and interaction between the different ingredients of asphalt concrete [11]. Abbas et al. and Liu and Dai conducted micromechanical modeling for asphalt concrete and analyzed the viscoelastic behavior of asphalt concrete based on discrete element method [12, 13]. Collop et al. performed uniaxial compressive creep test simulation for asphalt concrete based on elastic contacting model [14]. Based on the combination of DEM and image processing technology, You et al. built threedimensional DEM model of asphalt concrete and simulated the dynamic modulus test of asphalt concrete to predict the compressible dynamic moduli of asphalt concrete [15] and Khattak and Roussel and Khattak et al. developed a twodimensional DEM model of asphalt concrete to analyze the strength and dynamic modulus of asphalt concrete under indirect tension mode [16, 17]. Based on random modeling algorithm for asphalt concrete, Zhang et al. and Hou et al. investigated the micromechanical response of asphalt concrete under loading pressure and analyzed the rutting property and mechanism of asphalt concrete [18, 19]. Buttlar et al. and Kim et al. investigated the tension failure behavior and fracture energy by simulating the singleedge notched beam test and diskshaped compact tension test [20, 21]. Kim and Buttlar studied the discrete fracture modeling for asphalt concrete and investigated the fracture behavior of asphalt concrete [22, 23]. Yang et al. simulated the bending beam fracture test by adopting discrete element method and analyzed the healing property of asphalt concrete by using bond healing model [24]. Chen et al. investigated both the dynamic behavior and the fracture behavior of asphalt concrete by simulating the creep test and splitting test of asphalt concrete [25, 26].
However, few researches were performed to evaluate and analyze the lowtemperature cracking behavior based on threedimensional discrete element modeling and the impacts by air voids on the lowtemperature properties of asphalt concrete. This study focused on the impacts of different parameters of air voids on the lowtemperature properties of densegraded asphalt concrete. DEM and PFC3D were used to build threedimensional digital sample and virtual lowtemperature bending beam test for densegraded asphalt concrete based on laboratory tests. And the influences of air void content, distribution of air voids, and size of single air void on the lowtemperature properties of asphalt concrete were analyzed.
2. Materials and Experimental Test
2.1. Materials
A 13 mm densegraded asphalt concrete (AC13) with nominal maximum aggregate size of 13.2 mm, which was widely used as the wearing course in China, was prepared for laboratory test and micromechanical modeling. The mix design of AC13 satisfied the specifications set forth by Chinese Ministry of Transportation and is shown in Table 1. If all of the aggregates especially the fine aggregates and mineral fillers were considered during micromechanical modeling for asphalt concrete, it is too timeconsuming to generate virtual sample and conduct the virtual test during PFC3D. Thus, to facilitate micromechanical modeling in PFC3D, asphalt concrete was considered as a threephase composition that consisted of three ingredients which are air voids, asphalt mortar composed of asphalt binder and fine aggregates passing 2.36 mm sieving size, and coarse aggregates retained on 2.36 mm sieving size.

2.2. Experimental Tests
The lowtemperature threepoint bending beam test was performed for AC13 by Universal Testing Machine (UTM). The testing temperature was −10°C. And loading was applied by cylindrical pressure bar with diameter of 2 cm on the span center of the beam sample with dimensions of 250 × 30 × 35 mm^{3} (length × width × height) at loading speed of 50 mm/min until the beam was ruptured. Based on the rupture load and the rupture displacement at the span center of beam sample immediately after the sample was ruptured, the fracture tensile stress, fracture tensile strain, and fracture strain energy density can be obtained and recorded. The lowtemperature splitting test was conducted at −10°C for asphalt mortar. During the splitting test, loading was applied on the cylindrical sample with height of 63.5 mm and diameter of 101.6 mm at loading speed of 50 mm/min until the sample was split to get the splitting tensile stress and splitting tensile modulus for mortar sample. Figure 1 shows the test samples for the lowtemperature threepoint bending beam test and lowtemperature splitting test, respectively.
(a)
(b)
3. Discrete Element Modeling for Virtual Test
3.1. Micromechanical Models and Parameters
During PFC3D modeling, the microstructure of asphalt concrete was modeled as a threeingredient system (coarse aggregates, asphalt mortar, and air voids) and different contact models were used to describe the micromechanical behavior of different ingredients. Based on PFC3D manual [27], the contact models at different contacts within asphalt concrete are summarized in Table 2.

The micromechanical parameters for different contact models can be determined by the macromechanical properties of coarse aggregates and asphalt mortar [27], as shown in the following: where , , and are the normal stiffness, shear stiffness, and friction coefficient at contacts between aggregates; , , and are the normal stiffness, shear stiffness, and maximum tensile force at contacts within asphalt mortar; , , and are the normal stiffness, shear stiffness, and maximum tensile force at contacts within asphalt mortar; is the radius of the discrete ball element for aggregate and asphalt mortar which is 1 mm in this study; , , and are the elastic modulus, Poisson ratio, and friction coefficient of aggregates; and and are the tensile modulus and strength from splitting test of asphalt mortar.
Based on previous research [15, 26], the elastic modulus and friction coefficient of coarse aggregates are presented in Table 3. Based on splitting tests of asphalt mortar, the tensile stress and modulus of asphalt mortar are also summarized in Table 3. According to (1), the micromechanical modeling parameters at different contacts within asphalt concrete are determined and presented in Table 4.


3.2. Micromechanical Modeling of Virtual Test
During micromechanical modeling by PFC3D, asphalt mortar was modeled by discrete ball elements with the same size, and air voids were considered to be distributed within asphalt mortar randomly and simulated by removing elements of asphalt mortar randomly to meet the designed air void content of asphalt concrete. However, PFC3D cannot generate irregular elements directly; thus, a userdefined modeling algorithm was performed in PFC3D to get polyhedrons with irregular shapes to simulate coarse aggregates. Based on the previous assumptions and the testing conditions of laboratory lowtemperature bending beam test, as shown in Figure 2, a micromechanical modeling procedure was proposed to build virtual lowtemperature bending beam test. Figure 3 shows the critical generation process during PFC3D modeling for virtual lowtemperature bending beam test.
(a)
(b)
(c)
(d)
(e)
(f)
4. Results and Discussion
4.1. Validity Verification of Virtual Test
The laboratory bending beam test was conducted to verify the reliability of the virtual bending beam test. The failure sample from the laboratory test is shown in Figure 4 while Figure 5 illustrates the different testing stages during virtual test. It can be seen that the virtual test can capture the developing process of cracking failure which is very similar to the cracking failure of the laboratory test. Figure 6 shows the test curves from laboratory test and virtual test. It can be seen that the testing curve of virtual test is similar to the testing curve of laboratory test. It proves the validity of using virtual bending beam test to predict the lowtemperature property of asphalt concrete.
(a)
(b)
(c)
(d)
(e)
4.2. Effects by Content of Air Voids on LowTemperature Property
Based on the built modeling process, as shown in Figure 7, beam samples with different contents of air voids (2%, 4%, 6%, 8%, and 10%) were built for virtual lowtemperature bending beam test to analyze the influences by air void content on the lowtemperature properties of asphalt concrete. The changing of tensile failure strength and failure strain with variation of air void contents are shown in Figure 8. It can be seen that all of the three indices including failure strength, failure strain, and strain energy density decrease with the air void contents increasing, especially for the strain energy density. It indicates that the lowtemperature property of asphalt concrete gets worse with its air void content growing. When the air void content exceeds 6% especially, the degradation of lowtemperature property becomes more serious. It well confirms with the idea that the common mix design of asphalt concrete tends to keep the target air void content lower than 6%.
(a)
(b)
(c)
(d)
(e)
(a)
(b)
(c)
4.3. Effects by Air Voids Distribution on LowTemperature Property
During the virtual bending beam test, while the total content of air voids of test sample was kept as 4%, the nonuniform vertical distribution and nonuniform horizontal distribution of air voids in test sample were simulated, respectively, as shown in Figures 9 and 10. In Figure 9, along the vertical direction, the samples were cut apart into two parts with equal volume. Five different air void content distributions, which are 8% in the upper part and 0% in the lower part (V8/0), 6% in the upper part and 2% in the lower part (V6/2), 4% in the upper part and 4% in the lower part (V4/4), 2% in the upper part and 6% in the lower part (V2/6), and 0% in the upper part and 8% in the lower part (V0/8), were generated. In Figure 10, along the horizontal direction, the samples were cut apart into three parts with the same volume. Six different air void content distributions, which are 0% in the side parts and 12% in the middle parts (H0/12/0), 1% in the side parts and 0% in the middle part (H1/10/1), 2% in the side parts and 8% in the middle part (H2/8/2), 4% in all of the three parts (H4/4/4), 5% in the side parts and 2% in the middle part (H5/2/5), and 6% in the side parts and 0% in the middle part (H6/0/6), were considered.
(a)
(b)
(c)
(d)
(e)
(a)
(b)
(c)
(d)
(e)
(f)
Figures 11 and 12 show the testing results of asphalt concrete samples with different nonuniform air voids distribution. It is indicated that different air voids distributions within the samples result in different lowtemperature properties. From Figure 11(a), it can be seen that the failure strength increases with the air void content of bottom lower part declining. From Figures 11(b) and 11(c), it is shown that the sample with uniform distribution of air voids has the biggest failure strain and strain energy density; besides that both the failure strain and strain energy density increase with the air void content of lower part declining. It indicates that the air void content variation of lower part has more influences on the lowtemperature property than that of the upper part. From Figure 12, it is shown that all of the three indices decrease with the air void content of middle part growing. When the air void content of middle part exceeds 6% especially, the degradation of all of the three indices becomes more sharp. Since the loading was applied in the center of the middle part, it confirms well with the previous analysis about the influences by air void contents on the lowtemperature properties. Thus, the variation of air void content within the middle part has important impacts on the lowtemperature property of the testing sample.
(a)
(b)
(c)
(a)
(b)
(c)
4.4. Effects by Air Void Size on LowTemperature Property
To analyze the effects by air void size on the lowtemperature property, different numbers of asphalt mortar elements contacting with each other were removed to get air voids with different sizes. During PFC3D modeling, four different air void sizes were modeled by removing mortar element (named Size 1), two interconnected mortar elements (named Size 2), three interconnected mortar elements (named Size 3), and four interconnected mortar elements (named Size 4). As shown in Figure 13, while the total air void content was kept as 4%, samples with different single air void sizes were built for virtual bending beam tests. The testing results are shown in Figure 14. It can be seen that all of the three indices decline with the air void size growing. It is shown that smaller air void size of asphalt concrete results in better lowtemperature property of asphalt concrete.
(a)
(b)
(c)
(d)
(a)
(b)
(c)
5. Conclusions
Micromechanical modeling procedure based on discrete element method and PFC3D was built to simulate the lowtemperature bending beam test in laboratory. Based on laboratory testing data, the validity of virtual test to characterize the lowtemperature property of asphalt concrete was proved. It provides an effective method to analyze the impacts by air voids on the lowtemperature properties of densegraded asphalt concrete which are difficult to be carried out by laboratory tests.
It is proved that the growing of air void content weakens the lowtemperature properties of densegraded asphalt concrete, especially when the content of air voids is bigger than the designed content of air voids. Even with the same mix design and content of air voids, asphalt concrete can still exhibit very different lowtemperature properties. Nonuniform air voids distribution and air void sizes variation have important impacts on the lowtemperature properties of asphalt concrete, especially when the air void content and size within the loading area of asphalt concrete vary. Therefore, lower air void content, uniform distribution of air voids, and small size of interconnected air voids are helpful to improve the lowtemperature properties of asphalt concrete.
Future study will focus on different types of asphalt concretes such as stone matrix asphalt concrete and porous asphalt concrete, different types of air voids such as impermeable void and permeable void, and the relationship between volumetric characteristics and asphalt concrete behaviors.
Competing Interests
The authors declare no competing interests regarding the publication of this paper.
Acknowledgments
The study is financially supported by the National Natural Science Foundation of China (no. 51378006), National Science and Technology Support Program (2014BAG05B04), Huoyingdong Foundation of the Ministry of Education of China (no. 141076), Excellent Young Teacher Program of Southeast University (2242015R30027), Natural Science Foundation of Jiangsu (BK20161421 and BK20140109), State Key Laboratory of High Performance Civil Engineering Materials (2014CEM008), and National Engineering Laboratory for Surface Transportation Weather Impacts Prevention (NELLM201604).
References
 Y. Q. Zhang, R. Luo, and R. L. Lytton, “Mechanistic modeling of fracture in asphalt mixtures under compressive loading,” Journal of Materials in Civil Engineering, vol. 25, no. 9, pp. 1189–1197, 2013. View at: Publisher Site  Google Scholar
 Y. Zhang, X. Luo, R. Luo, and R. L. Lytton, “Crack initiation in asphalt mixtures under external compressive loads,” Construction and Building Materials, vol. 72, pp. 94–103, 2014. View at: Publisher Site  Google Scholar
 J. Chen, H. Wang, and L. Li, “Virtual testing of asphalt mixture with twodimensional and threedimensional random aggregate structures,” International Journal of Pavement Engineering, 2015. View at: Publisher Site  Google Scholar
 J. Chen, M. Zhang, H. Wang, and L. Li, “Evaluation of thermal conductivity of asphalt concrete with heterogeneous microstructure,” Applied Thermal Engineering, vol. 84, pp. 368–374, 2015. View at: Publisher Site  Google Scholar
 H. Wang, J. Wang, and J. Q. Chen, “Micromechanical analysis of asphalt mixture fracture with adhesive and cohesive failure,” Engineering Fracture Mechanics, vol. 132, pp. 104–119, 2014. View at: Publisher Site  Google Scholar
 J. P. Zhang, J. Pei, and Z. Zhang, “Development and validation of viscoelasticdamage model for threephase permanent deformation of dense asphalt mixture,” Journal of Materials in Civil Engineering, vol. 24, no. 7, pp. 842–850, 2012. View at: Publisher Site  Google Scholar
 Y. Zhang, B. Birgisson, and R. Lytton, “Weak form equation—based finiteelement modeling of viscoelastic asphalt mixtures,” Journal of Materials in Civil Engineering, vol. 28, no. 2, Article ID 04015115, pp. 1–13, 2016. View at: Publisher Site  Google Scholar
 Q. Dai and Z. You, “Prediction of creep stiffness of asphalt mixture with micromechanical finiteelement and discreteelement models,” Journal of Engineering Mechanics, vol. 133, no. 2, pp. 163–173, 2007. View at: Publisher Site  Google Scholar
 P. A. Cundall, “A computer model for simulating progressive large scale movements in blocky rock systems,” in Proceedings of the Symposium of International Society of Rock Mechanics, vol. 1, pp. 2–8, Nancy, France, 1971. View at: Google Scholar
 P. A. Cundall and O. D. L. Strack, “A discrete numerical model for granular assemblies,” Géotechnique, vol. 29, no. 1, pp. 47–65, 1979. View at: Publisher Site  Google Scholar
 W. G. Buttlar and Z. P. You, “Discrete element modeling of asphalt concrete: a microfabric approach,” Transportation Research Record, vol. 1757, pp. 111–118, 2001. View at: Publisher Site  Google Scholar
 A. Abbas, E. Masad, T. Papagiannakis, and T. Harman, “Micromechanical modeling of the viscoelastic behavior of asphalt mixtures using the discreteelement method,” International Journal of Geomechanics, vol. 7, no. 2, pp. 131–139, 2007. View at: Google Scholar
 Y. Liu and Q. Dai, “Viscoelastic model for discrete element simulation of asphalt mixtures,” Journal of Engineering Mechanics, no. 4, pp. 324–333, 2009. View at: Google Scholar
 A. C. Collop, G. R. McDowell, and Y. Lee, “Use of the distinct element method to model the deformation behavior of an idealized asphalt mixture,” International Journal of Pavement Engineering, vol. 5, no. 1, pp. 1–7, 2004. View at: Google Scholar
 Z. You, S. Adhikari, and Q. Dai, “Threedimensional discrete element models for asphalt mixtures,” Journal of Engineering Mechanics, vol. 134, no. 12, pp. 1053–1063, 2008. View at: Publisher Site  Google Scholar
 M. J. Khattak and C. Roussel, “Micromechanical modeling of hotmix asphalt mixtures by imaging and discrete element methods,” Transportation Research Record, no. 2127, pp. 98–106, 2009. View at: Google Scholar
 M. J. Khattak, A. Khattab, H. R. Rizvi, S. Das, and M. R. Bhuyan, “Imagedbased discrete element modeling of hot mix asphalt mixtures,” Materials and Structures, no. 48, pp. 2417–2430, 2015. View at: Google Scholar
 D. Zhang, X. Huang, and Y. Zhao, “Algorithms for generating threedimensional aggregates and asphalt mixture samples by the discreteelement method,” Journal of Computing in Civil Engineering, vol. 27, no. 2, pp. 111–117, 2013. View at: Publisher Site  Google Scholar
 S. Hou, D. Zhang, X. Huang, and Y. Zhao, “Investigation of micromechanical response of asphalt mixtures by a threedimensional discrete element model,” Journal of Wuhan University of Technology: Materials Science Edition, vol. 30, no. 2, pp. 338–343, 2015. View at: Publisher Site  Google Scholar
 W. G. Buttlar, H. Kim, and M. P. Wagoner, “Toward realistic heterogeneous fracture modeling of asphalt mixture using diskshaped compact tension test based on discontinuum approach,” in Proceedings of the CDROM of the Transportation Research Board 85th Annual Meeting, no. 062975, pp. 1–23, Washington, DC, USA, 2006. View at: Google Scholar
 H. Kim, M. P. Wagoner, and W. G. Buttlar, “Micromechanical fracture modeling of asphalt concrete using a singleedge notched beam test,” Materials and Structures, vol. 42, article 677, 2009. View at: Publisher Site  Google Scholar
 H. Kim and W. G. Buttlar, “Discrete fracture modeling of asphalt concrete,” International Journal of Solids and Structures, vol. 46, no. 13, pp. 2593–2604, 2009. View at: Publisher Site  Google Scholar
 H. Kim and W. G. Buttlar, “Multiscale fracture modeling of asphalt composite structures,” Composites Science and Technology, vol. 69, no. 2, pp. 2716–2723, 2009. View at: Publisher Site  Google Scholar
 X. Yang, Q. Dai, Z. You, and Z. Wang, “Integrated experimentalnumerical approach for estimating asphalt mixture induction healing level through discrete element modeling of a singleedge notched beam test,” Journal of Materials in Civil Engineering, vol. 27, no. 9, Article ID 04014259, 2008. View at: Publisher Site  Google Scholar
 J. Chen, T. Pan, and X. Huang, “Discrete element modeling of asphalt concrete cracking using a userdefined threedimensional micromechanical approach,” Journal of Wuhan University of Technology: Materials Science Edition, vol. 26, no. 6, pp. 1215–1221, 2011. View at: Publisher Site  Google Scholar
 J. Chen, T. Pan, J. Chen, X. Huang, and Y. Lu, “Predicting the dynamic behavior of asphalt concrete using threedimensional discrete element method,” Journal of Wuhan University of TechnologyMaterials Science Edition, vol. 27, no. 2, pp. 382–388, 2012. View at: Publisher Site  Google Scholar
 Itasca Consulting Group, PFC3D Version 4.0, Itasca Consulting Group, Minneapolis, Minn, USA, 2008.
Copyright
Copyright © 2016 Tao Ma et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.